FSC 9310 JCP Q20
RAILROAD BOARD, WHITE AND COLORED
Cardboard February 1, 1999
Use information: This paragraph is informational only and is not exclusively definitive of the end use.
For letterpress and offset printing of signs, display cards, cloth or paper-stripped covers, two-piece covers for use with bindings such
as plastic combs, wire-o, and spiral. Printed matter may include text, line illsutrations, and solid reverses.
Stock: Facing sheets shall be uncoated and shall not exceed 25 pct Color: The paper board in the order (or publication) shall be
groundwood pulp. uniform. The color variation shall not exceed DE(CIELAB)=1.0
Note: Not less than 80 pct total recovered fiber of which 15 per- with a target brightness of the white board not less than 79 pct.
centage points shall be postconsumer fiber. Postconsumer fiber, in For colored stock, board shall match one of the established
any percent over 15 percentage points, is encouraged, provided standards. Colors shall be ash gray, blue, buff, green, orange,
that the requirements of this Standard are met. red or as specified. The commercial color standard is applicable,
Thickness: Average (mm) ........................ 0.45 0.76 1.22 unless specified that the color shall conform to the Government
Equivalent (inch) .................................... 0.0180 0.0300 0.0480 standard. Colors shall not fade and shall appear even and uni-
Tolerance: Plus or minus (mm) ............. 0.026 0.050 0.065 form on the surface of the board.
Equivalent (inch) .................................... 0.001 0.002 0.0025
General appearance: The color and cleanliness shall conform to Sampling and testing: Shall be conducted in accordance with
the standard sample(s) adopted by the Government. standards in Part 2, Government Paper Specification Standards.
Unless otherwise specified, the following is automatically waived when printing or duplicating is to be accomplished on commercial contract
Curl: Paper board shall lie flat with either no tendency to curl or Paper board with the long dimension 813 mm (32 inches) or less
with a curl which can be overcome under reasonable working shall be considered square if the variation does not exceed 1 mm
conditions. (1⁄32 inch); over 813 mm (32 inches), 2 mm (1⁄16 inch).
Size and trim: Paper board shall be furnished in the size(s) or- Grain: Direction of the grain on flat board shall be as ordered.
dered and shall be flat, trimmed square on four sides with clean
smooth edges, and evenly jogged. A tolerance of ±2 mm (1⁄16 Pressroom conditions: The bulk of this paper board will be used
inch) shall be allowed. Successive sheets within any package in air-conditioned pressrooms maintained at 24 °C ±2 °C and
shall not differ from each other by more than 0.5 mm (1⁄64 inch). 45 pct ±8 pct relative humidity.